advertisement

Hindawi Publishing Corporation Journal of Nanomaterials Volume 2011, Article ID 746029, 9 pages doi:10.1155/2011/746029 Research Article Fracture Toughness of Carbon Nanotube-Reinforced Metal- and Ceramic-Matrix Composites Y. L. Chen,1, 2 B. Liu,1 Y. Huang,3 and K. C. Hwang1 1 AML, Department of Engineering Mechanics, Tsinghua University, Beijing 100084, China of Mechanical Engineering, The Ohio State University, Columbus, OH 43210, USA 3 Department of Civil and Environmental Engineering and Department of Mechanical Engineering, Northwestern University, Evanston, IL 60208, USA 2 Department Correspondence should be addressed to B. Liu, [email protected] Received 15 July 2010; Accepted 1 November 2010 Academic Editor: Teng Li Copyright © 2011 Y. L. Chen et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Hierarchical analysis of the fracture toughness enhancement of carbon nanotube- (CNT-) reinforced hard matrix composites is carried out on the basis of shear-lag theory and facture mechanics. It is found that stronger CNT/matrix interfaces cannot definitely lead to the better fracture toughness of these composites, and the optimal interfacial chemical bond density is that making the failure mode just in the transition from CNT pull-out to CNT break. For hard matrix composites, the fracture toughness of composites with weak interfaces can be improved eﬀectively by increasing the CNT length. However, for soft matrix composite, the fracture toughness improvement due to the reinforcing CNTs quickly becomes saturated with an increase in CNT length. The proposed theoretical model is also applicable to short fiber-reinforced composites. 1. Introduction Carbon nanotubes (CNTs) possess exceptionally superior physical and mechanical properties, such as high strength, low density, high flexibility, and high toughness and therefore hold great promise for employment as reinforcements in advanced composites [1–10]. However, experimental and numerical studies show that the performance of such composites depends critically on the CNT/matrix interfacial characteristics [11–13]. Interface strength and interface length are two of the most important factors that aﬀect the mechanical properties of CNT-reinforced composites and therefore have drawn the attention of many researchers. As a type of extraordinary reinforcements, CNTs can be incorporated in a polymer, metal, or ceramic matrix. The focus of many previous studies in CNT-reinforced composites has been on polymer-matrix materials [14– 21], and researchers have tried in various ways, such as nonionic surfactant and ion bombardment [11, 16, 22, 23], to form covalent bonds between CNTs and the polymer matrix to strengthen the interface. In order to know whether longer CNTs and stronger interfaces definitely result in better mechanical properties of CNT-reinforced composites, Chen et al. [24] studied the fracture toughness enhancement of CNT-reinforced polymer-matrix composites. They found that neither longer reinforcing CNTs nor stronger CNT/matrix interfaces can definitely lead to the better fracture toughness, and the optimal interfacial chemical bond density and the optimal CNT length are those making the failure mode just in the transition from CNT pull-out to CNT break. Meanwhile, the production and application of CNTreinforced metal- and ceramic-matrix composites draw more and more attention. Ma and coworkers [25] formed CNTnano-silicon-carbide (SiC)/ceramic composites and reported a 10% improvement in the strength and fracture toughness as compared to the monolithic ceramics. These modest improvements are attributed to nanotube/matrix debonding and crack deflection. The techniques to form CNT/metaloxide composites as well as CNT/metal-matrix composites have been developed [26–31]. However, they did not provide the expected improvement in mechanical properties. Is Chen et al.’s conclusion [24] still valid for these hard matrix composites? Is there some diﬀerence between the soft matrix 2 Journal of Nanomaterials and hard matrix CNT-reinforced composites? This paper will focus on the case with higher matrix stiﬀness and study the influence factors on the fracture toughness of CNTreinforced composites. the critical shear displacement δb , which depends only on the type of functionalization bond at the interface, whereas the corresponding interface strength τb also depends on the interface bond density. The interface shear stress τ is assumed to be proportional to the relative displacement Δu, that is, 2. Roadmap for Hierarchical Failure Analysis of CNT-Reinforced Composites τ(x) = kΔu(x) = k um (x) − u f (x) , In CNT-reinforced composites with macroscopic cracks, the high strength of CNTs can retard crack propagation, and a fracture zone bridged by CNTs at the crack tip is formed, as shown in Figure 1(a). This toughening eﬀect of bridging CNTs is equivalent to that of nonlinear springs connecting the upper and lower crack surfaces, as shown in Figure 1(b). The force-displacement relation for these springs can be obtained by studying the pulling force F and pull-out displacement δ of a single CNT, as in Figure 1(c). This F − δ curve depends on the interfacial atomic bond properties, that is, on the interaction between atoms, as shown in Figure 1(d). Therefore, CNT-reinforced composites have three failure mode levels: a bond break at the atomistic level, CNT fiber failure mode at the mesoscopic level, and macroscopic crack propagation at the macroscopic level. To better understand and optimize the toughness of CNT-reinforced composites, this paper presents hierarchical failure analysis. We first adopt shear-lag theory to investigate CNT fiber in Section 3 and then use facture mechanics to study macroscopic-level failure in Section 4. Our conclusions are summarized in the last section. 3. Force-Displacement Relation of a Single CNT Pulled from the Matrix There are a large number of continuum mechanics studies on the fiber-reinforced composites, especially the widely used shear-lag theory [32–37]. Chon and Sun [33] studied stress distribution along a single reinforcing fiber of a randomly oriented chopped-fiber composite under the assumption of perfect bonding. Lawrence [34] assumed the stiﬀness of the fiber is lower than that of the matrix and investigated fiber pull-out from an elastic matrix. For ceramic composites, Marshall et al. [35] studied the cracking in brittle matrix. Hutchinson and Jensen [36] treated debonding process as a mode 2 crack to study fiber debonding and pull-out, and based on these studies, Budiansky et al. [37] accounted for an interfacial debonding resistance and studied the eﬀects of debonding and initial stress on overall composite toughness. Many of these models are also applicable to CNT-reinforced composites. However, for the completeness and convenience to readers, the related analysis is still briefly presented in this section. where k = τb /δb is the shear stiﬀness of the interface and um (x) and u f (x) are the axial or x-direction displacements of the matrix and the CNT fiber, respectively. Suppose the CNT and the matrix are both linear elastic, with Young’s modulus E f and Em , respectively. A representative volume element (RVE) including a single CNT with embedded length L and diameter d, as shown in Figure 2, is adopted for analysis. With the balance conditions of the fiber and the matrix, the shear stress distribution can be derived [24] τ(x) = F τb Cδb · sinh L Cτb /δb + 1/(Em Am ) cosh x Cτb /δb (2) 1/ E f A f cosh (x − L) Cτb /δb sinh L Cτb /δb , where A f and Am are the cross-section areas of the CNT and the matrix in the RVE, F is the pulling force, and C depends on the material constants and geometry parameters as C = πd 1 1 + . E f A f Em Am (3) The distribution of the axial normal stress in the CNT can also be derived as 1 F− σ(x) = Af x 0 πdτ(x)dx . (4) 3.2. Critical Pull-Out/Break Condition of CNTs. The two main fiber-level failure modes are usually interfacial debonding and fiber break, depending on the interfacial shear stress and the axial normal stress, respectively. When the composite is under increasing tension, both the shear stress on the interface and the axial normal stress in the CNT increase. 3.2.1. Critical Condition for CNT Fiber Break. Obviously, the maximum axial normal stress in the CNT is located at position x = 0 and can be expressed as σ(x)|max = σ(0) = 3.1. Shear-Lag-Model-Based Stress Analysis of the CNT and Matrix. According to the shear-lag theory, the interaction between the CNTs and the matrix that results from the chemical bonds shown in Figure 2 is shear stress, which is related to the relative displacement between the CNT fiber and the matrix Δu. A bond break occurs when Δu reaches (1) F . Af (5) CNT break occurs when the maximum axial normal stress reaches CNT strength σ bf , and the corresponding critical pulling force is σ = σ bf A f . Fmax (6) Journal of Nanomaterials 3 K∞ (a) F K∞ Δu τ F (b) Macroscopic level Δu δb δ (c) Mesoscopic level (d) Atomistic level Figure 1: Schematic diagram of three-level failure analysis models. (a) Fracture zone bridged with CNTs at the crack tip. (b) Macroscopiclevel model with equivalent bridging nonlinear springs. (c) Mesoscopic-level model for studying CNT-fiber failure and obtaining the forcedisplacement relation of equivalent nonlinear spring. (d) Atomistic-level failure model for characterizing CNT/matrix interfacial bond breaking. L Matrix Am F Af CNT o d x (b) (a) Figure 2: Schematic diagram of shear-lag model for the interactions between the CNT and the matrix (a), and the geometric parameters (b). 3.2.2. Critical Condition for Interfacial Debonding. According to (2), the maximum shear stress on the interface may appear at either x = 0 for E f A f < Em Am or x = L for E f A f > Em Am . In CNT/polymer composites, the stiﬀness of the CNT is usually greater than that of the matrix, that is, E f A f > Em Am , as Chen et al. have previously discussed in [24], but in metal- and ceramic-matrix composites Young’s modulus of the matrix is close to that of the CNTs, so the stiﬀness of the CNT is less than that of the matrix, that is, E f A f < Em Am . The current paper is focused on this hard matrix regime and sometimes also presents the results of soft matrix regime for comparison. (1) E f A f < Em Am Case (Hard Matrix). From (2), the maximum shear stress on the interface can be found at the x = 0 position, and τ(x)|max = τ(0) =F τb Cδb · 1/(Em Am ) + 1/ E f A f cosh L Cτb /δb sinh L Cτb /δb (7) . 4 Journal of Nanomaterials where α = Em Am /(E f A f ) is the stiﬀness ratio of the matrix to the CNT, and The corresponding critical pulling force is τ0 Fmax = Cτb δb sinh L Cτb /δb 1/(Em Am ) + 1/ E f A f cosh L Cτb /δb . Together with (6) and (8), the transition condition between the pull-out and break failure modes is σ bf A f 1/(Em Am ) + 1/ E f A f cosh L Cτb /δb Cτb δb sinh L Cτb /δb σ bf A f Cτb δb sinh L Cτb /δb >1 <1 CNT fiber breaking , (2) E f A f > Em Am Case (Soft Matrix). The most important diﬀerence from the hard matrix case (i.e., E f A f < Em Am ) is that the maximum shear stress on the interface is found at the x = L position, so the critical pulling force is [24] τL Fmax = Cτb δb sinh L Cτb /δb , (10) δCτ0 = δb . Cτb δb sinh L Cτb /δb F(L2 ) = Cτb δb · Cτb δb sinh L Cτb /δb cosh L2 Cτb /δb + 1/α , sinh L2 Cτb /δb ⎞ ⎠. cosh L2 Cτb /δb + 1/α (15) Getting rid of L2 from the above two equations, we can get the relation between the pulling force F and the pull-out displacement δ after the beginning of interface debonding as >1 (11) E f A f sinh L2 Cτb /δb ⎛ δ(L2 ) = δb + (L − L2 )⎝ Cτb δb · ⎧ ⎪ ⎪ ⎨ interfacial debonding, σ bf A f 1/(Em Am ) cosh L Cτb /δb + 1/ E f A f (14) At this time, the relative displacement at the x = L position is δb · (1/α)(1 + (α2 − 1)/(α cosh(L Cτb /δb ) + 1)), which is less than δb , so the interface is not debonded completely and can still stand some degree of shear stress. After this point, the F − δ curve decreases until the interface debonds completely. In the process of debonding, the CNT and the matrix can be analyzed as a similar system but with a shorter interface length L2 (L2 < L). Both the pulling force F and the pull-out displacement δ are dependent on the new interface length L2 as follows: and the transition condition between the pull-out and break failure modes is [24] σ bf A f 1/(Em Am ) cosh L Cτb /δb + 1/ E f A f (13) 3.3.2. Interface Debonding from the End of Pulling Force (Hard Matrix). If E f A f < Em Am , the interface begins to debond at the x = 0 position where the relative displacement reaches δb . So the critical pull-out displacement for the interfacial debonding case is 1/(Em Am ) cosh L Cτb /δb + 1/ E f A f δb . · Cτb E f sinh L Cτb /δb (9) that is, a weak interface results in interfacial debonding and fiber pull-out, whereas a strong interface leads to fiber break. δCσ = σ bf cosh L Cτb /δb + 1/α interfacial debonding , 1/(Em Am ) + 1/ E f A f cosh L Cτb /δb (8) <1 δ = δb + ⎪ L − ⎪ ⎩ ⎡ ⎤⎫ ⎪ F + F 2 + α2 Cτb δb E2f A2f − F 2 ⎥⎪ ⎬ δb ⎢ ⎢ ⎥ ln⎣ ⎦ ⎪ Cτb ⎪ α E f A f Cτb δb − F ⎭ F . × Ef Af CNT fiber breaking. (16) 3.3. Relation between Pulling Force and Pull-Out Displacement. For diﬀerent possible failure modes, there are three types of F − δ curves, as shown in Figures 3(a), 3(b), and 3(c). Here, F is the pulling force, and δ = Δu(0) is the pullout displacement. The corresponding relations are given as below. 3.3.1. CNT Break Case. The F − δ relation can be obtained as ⎧ ⎪ ⎪ Cτb ⎪ ⎨ F=⎪ ⎪ ⎪ δ ⎩0, δb · E f A f sinh L Cτb /δb So the relation between the pulling force F and the relative displacement δ is ⎧ ⎪ ⎪ Cτb ⎪ ⎨ F=⎪ ⎪ ⎪ δ ⎩F δb · E f A f sinh L Cτb /δb cosh L Cτb /δb + 1/α cosh L Cτb /δb + 1/α 0 ≤ δ ≤ δCσ , δ > δCσ , (12) , 0 ≤ δ ≤ δb , δb < δ ≤ δmax , (17) soften (δ), , where Fsoften (δ) is solved from (16) and the maximum pullout displacement δmax is determined by ∂δ(L2 ) = 0. ∂L2 (18) Journal of Nanomaterials 5 Strong interface σ Fmax Pulling force F This process is shown in Figure 3(b), and the critical point τ0 ) is given by (14) and (8), respectively. It is (δCτ0 , Fmax interesting to notice that after the initial debonding at x = 0, the interface first debonds gradually and steadily, with the gradual deceasing pulling force, but when the pullout displacement reaches δmax , the whole bonding interface debonds simultaneously and the pulling force drops down to zero suddenly. CNT breaking F 3.3.3. Interface Debonding from the End Away from Pulling Force (Soft Matrix). As discussed by Chen et al. in [24], if E f A f > Em Am , the F − δ relation is F δCσ ⎧ ⎪ E A sinh L Cτ /δ f f b b ⎪ Cτ b ⎪ ⎪δ · , ⎪ ⎪ ⎪ δb cosh L Cτb /δb + 1/α ⎨ F=⎪ " 2 # ⎪ ⎪ 2 # ⎪ ⎪ ⎪Em Am $ Cτb δb − δ , ⎪ ⎩ δ 1 − α2 0 0 ≤ δ ≤ δCτL , Pull-out displacement δ (a) δCτL b < δ ≤ δb , (19) τ0 Fmax Hard matrix weak interface where ⎛ ⎞ 1 − α2 ⎠. = δb · ⎝α + cosh L Cτb /δb + α (20) The F − δ curve is shown in Figure 3(c), and the critical τL ) is given by (20) and (10), respectively. point (δCτL , Fmax Diﬀerent from the other debonding case in Section 3.3.2, the interface debonds gradually and steadily, until it goes down to zero. Pulling force F δCτL E f A f < Em Am Interfacial debonding F F δCτ0 δmax Pull-out displacement δ 4. Macroscopic-Level Fracture Failure Analysis (b) 4.1. Fracture Toughness Enhancement ΔK. In CNT-reinforced composites, crack propagation is retarded by the pulling force of the CNTs at the crack surface, the so-called “bridge-toughening eﬀect.” The displacement of the crack surface (i.e., half of the crack opening displacement) is [38] √ 2r = ηKIC r, π (21) √ where r √is the distance to the crack tip and η = 2 2(1 − ν2m )/(Em π) depends only on Young’s modulus Em and Poisson’s ratio νm . According to (12), (17), and (19), for all diﬀerent types of failure modes, the pulling force F(δ) can be expressed as a function of the distance to the macroscopic crack tip r, that is, F(δ) = F(δ(r)) = F(r). The homogenized traction on the crack surface is then p(r) = F(r) A f + Am −1 , (22) and the fracture toughness enhancement ΔK can be computed as [39] ∞ √ 2p(r) ΔK = √ dr. 0 πr (23) τL Fmax Pulling force F 2 1 − ν2m KIC δ= Em Soft matrix weak interface F E f A f > Em Am Interfacial debonding F δCτL δb Pull-out displacement δ (c) Figure 3: The relation between the pulling force and the pullout displacement for the three CNT-fiber failure modes (a) CNT breaking, (b) interface failure with partial steady debonding when E f A f < Em Am , and (c) interface failure with steady debonding when E f A f > Em A m . Journal of Nanomaterials Interfacial debonding F ΔKpull out L−→∞ Fracture toughness enhancement ΔK Fracture toughness enhancement ΔK 6 F L Hard matrix weak interface 0 Interfacial debonding F F L Soft matrix weak interface 0 Interface length L Interface length L (a) CNT breaking F F L L ΔKbreak L−→∞ Hard matrix strong interface Fracture toughness enhancement ΔK Fracture toughness enhancement ΔK Interfacial debonding F F (b) CNT breaking F F L Interfacial debonding F ΔKbreak L−→∞ F Soft matrix strong interface L LC LC 0 0 Interface length L Interface length L (c) (d) Figure 4: Schematic diagram for the eﬀect of the interface length on the fracture toughness enhancement: (a) hard matrix, weak interface 2 2 2 A2 δ ). (c) hard matrix, strong interface τ > (σ b )2 /(CE2 δ ); (d) soft τb < (σ bf ) /(CE2f δb ). (b) soft matrix, weak interface τb < (Cσ bf A f ) /(Em b m b f f b 2 2 2 matrix, strong interface τb > (Cσ bf A f ) /(Em Am δb ). 4.2. Factors Aﬀecting the Fracture Toughness Enhancement ΔK. For the case of hard matrix (E f A f < Em Am ), the factors aﬀecting the fracture toughness enhancement ΔK are discussed below, and some results of soft matrix regime in [24] are also presented briefly for comparison. 2 For the case with strong interface τb > (σ bf ) /(CE2f δb ), as shown in Figure 4(c), a critical length LC exists and can be determined from the pull-out/break critical condition (9): LC = 4.2.1. Eﬀect of Interface Length L. From the pull-out/break 2 critical condition (9), we know that if τb < (σ bf ) /(CE2f δb ), the failure mode should always be the CNT pull-out, as shown in Figure 4(a). In this case, the fracture toughness enhancement ΔK increases with an increase in the interface length L infinitely. This phenomenon is diﬀerent from the case of weak interface in the soft matrix CNT-reinforced composites shown in Figure 4(b), in which an upper limit of the fracture toughness enhancement exists so any further lengthening of the CNTs improves the fracture toughness of the composites only slightly [24]. δb ln Cτb σ bf 2 − σ bf (α2 − 1) . (24) α E f Cτb δb − σ bf + Cτb δb αE f 2 When L < LC , the CNT is pulled out, and the fracture toughness enhancement ΔK increases with an increase in the interface length L. If L is further increased beyond the critical length LC , the failure mode is converted from CNT pull-out to CNT break and ΔK drops significantly. In this regime, the fracture toughness enhancement ΔK decreases with an increase in L and finally approaches the following value: ΔKbreak |L → ∞ = 2 σ bf A f 2δb . πCτb A f + Am ηKIC E f (25) Journal of Nanomaterials 7 Fracture toughness enhancement ΔK F L F L Hard matrix Fracture toughness enhancement ΔK CNT breaking Interfacial debonding F F CNT breaking F L F Interfacial debonding F Soft matrix L τbC 0 F τbC 0 Interface strength τb Interface strength τb (a) (b) It is interesting to note that, in this case, lengthening the interface beyond the critical length can even decrease the fracture toughness, which is very similar to the result shown is Figure 4(d) for the soft matrix CNT-reinforced composites [24]. 4.2.2. Eﬀect of Interface Strength τb . Another important factor aﬀecting the toughness enhancement is interface strength τb , and its eﬀect is shown in Figure 5(a). When τb is small, the failure mode is CNT pull-out, and the fracture toughness enhancement ΔK increases with an increase in τb . Further increasing τb beyond the critical interface strength τbc , which can be determined by the pull-out/break critical condition (9), leads the failure mode to be converted from CNT pull-out to CNT break, and ΔK drops significantly. In this regime, the toughness enhancement ΔK decreases with an increase in τb . This result agrees with the experimental and numerical studies of Xia et al.’s work on ceramic-matrix composites [40, 41], as well as the theoretical studies for soft matrix CNT-reinforced composites in Figure 5(b) [24]. Therefore, for CNTs with a given length, the maximum fracture toughness of the composite is achieved when τb is only slightly smaller than the critical interface strength τbc . 4.3. Optimization of Fracture Toughness Enhancement. In this subsection, we attempt to optimize the composite fracture toughness for the case of E f A f < Em Am by tailoring both the interface length L and interface strength τb , which is essentially a bivariate optimization problem. For convenience, we use another group of variables, normalized interface length %L = L Cτb /δb and τb , instead. According to (9), the maximum ΔK with a given %L can be achieved when τb = optimal τb ⎞2 ⎛ & % σ bf A f 1 + α cosh L % =⎝ ⎠ (Cδb ). (26) L Em Am sinh L % Figure 6 shows the normalized fracture toughness enhancement ΔK% = ΔK · (A f + Am )ηKIC /σ bf A f δb versus %L for Normalized fracture toughness enhancement ΔK% Figure 5: Schematic diagram for the eﬀect of the interface strength on the fracture toughness enhancement: (a) hard matrix; (b) soft matrix. 3 α = Em Am /(E f A f ) = 103 5 2 Hard matrix 2.5 2 Soft matrix α = Em Am /(E f A f ) = 0.1 1.5 0.5 1 0.9 0.5 0 1 2 3 4 5 % Normalized interface length L 6 7 Figure 6: The normalized fracture toughness enhancement ΔK% as a function of the normalized interface length %L with diﬀerent stiﬀness ratio α = Em Am /(E f A f ) and optimal interface strength. cases with diﬀerent stiﬀness ratios: α = Em Am /(E f A f ). It % → ∞, ΔK reaches an infinite value. is found that when L And according to (26), the corresponding optimal interface strength is ' optimal ' '% τb L→∞ 2 α σ bf A f . = πdδb E f (α + 1) (27) This result is diﬀerent from the case of E f A f > Em Am studied by Chen et al. [24], which presents the upper limit of the fracture toughness enhancement, as shown in Figure 6 with the dashed lines. When E f A f < Em Am , the value of the dimensionless fracture toughness enhancement ΔK% increases % unlimitedly, as shown in Figure 6 by the solid lines. So, with L there is neither upper limit for ΔK% nor optimal value for the CNT length L. The optimal CNT length L can only depend 8 on the preparation level and some other factors such as the critical CNT length for clustering and self-folding [42]. 5. Conclusions Combining the shear-lag model and fracture mechanics, we have carried out the hierarchical failure analysis on CNT-reinforced composites with hard matrix. The following conclusions have been reached. (1) Stronger CNT/matrix interfaces cannot definitely lead to a better fracture toughness of these composites. In contrast, the optimal interfacial chemical bond density is that making the failure mode just in the transition from CNT pull-out to CNT break. (2) For composites with hard matrix, there exists a critical interface strength, below which the CNT is always pulled out, and the fracture toughness can be eﬀectively improved by increasing the interface length L. However, for soft matrix composite, the fracture toughness improvement due to the reinforcing CNTs quickly becomes saturated with an increase in CNT length. It should be noted that the theoretical analysis and conclusions drawn in this paper can also be extended to fiberreinforced composites. Acknowledgments The authors acknowledge the support of the National Natural Science Foundation of China (Grant nos. 10702034, 10732050, 90816006 and 10820101048) and the National Basic Research Program of China (973 Program), Grant nos. 2007CB936803 and 2010CB832701. References [1] M. M. J. Treacy, T. W. Ebbesen, and J. M. Gibson, “Exceptionally high Young’s modulus observed for individual carbon nanotubes,” Nature, vol. 381, no. 6584, pp. 678–680, 1996. [2] E. W. Wong, P. E. Sheehan, and C. M. Lieber, “Nanobeam mechanics: elasticity, strength, and toughness of nanorods and nanotubes,” Science, vol. 277, no. 5334, pp. 1971–1975, 1997. [3] M.-F. Yu, O. Lourie, M. J. Dyer, K. Moloni, T. F. Kelly, and R. S. Ruoﬀ, “Strength and breaking mechanism of multiwalled carbon nanotubes under tensile load,” Science, vol. 287, no. 5453, pp. 637–640, 2000. [4] B. Vigolo, A. Penicaud, C. Coulon et al., “Macroscopic fibers and ribbons of oriented carbon nanotubes,” Science, vol. 290, no. 5495, pp. 1331–1334, 2000. [5] B. I. Yakobson, M. P. Campbell, C. J. Brabec, and J. Bernholc, “High strain rate fracture and C-chain unraveling in carbon nanotubes,” Computational Materials Science, vol. 8, no. 4, pp. 341–348, 1997. [6] G. Gao, T. Çaǧin, and W. A. Goddard III, “Energetics, structure, mechanical and vibrational properties of singlewalled carbon nanotubes,” Nanotechnology, vol. 9, no. 3, pp. 184–191, 1998. [7] Y. L. Chen, B. Liu, J. Wu, Y. Huang, H. Jiang, and K. C. Hwang, “Mechanics of hydrogen storage in carbon nanotubes,” Journal of the Mechanics and Physics of Solids, vol. 56, no. 11, pp. 3224– 3241, 2008. Journal of Nanomaterials [8] Y. Yin, Y. L. Chen, J. Yin, and K. Huang, “Geometric conservation laws for Y-branched carbon nanotubes,” Nanotechnology, vol. 17, pp. 1–5, 2006. [9] Y.-L. Chen, B. Liu, Y.-J. Yin, Y.-G. Huang, and K.-C. Hwuang, “Nonlinear deformation processes and damage modes of super carbon nanotubes with armchair-armchair topology,” Chinese Physics Letters, vol. 25, no. 7, pp. 2577–2580, 2008. [10] Y. Chen, Y. Yin, Y. Huang, and K.-C. Hwang, “Atomistic simulations of the nonlinear deformation and damage modes of super carbon nanotubes,” Journal of Computational and Theoretical Nanoscience, vol. 6, no. 1, pp. 41–45, 2009. [11] F. H. Gojny, J. Nastalczyk, Z. Roslaniec, and K. Schulte, “Surface modified multi-walled carbon nanotubes in CNT/epoxycomposites,” Chemical Physics Letters, vol. 370, no. 5-6, pp. 820–824, 2003. [12] S. J. V. Frankland, A. Caglar, D. W. Brenner, and M. Griebel, “Molecular simulation of the influence of chemical cross-links on the shear strength of carbon nanotube-polymer interfaces,” Journal of Physical Chemistry B, vol. 106, no. 12, pp. 3046– 3048, 2002. [13] S. J. V. Frankland and V. M. Harik, “Analysis of carbon nanotube pull-out from a polymer matrix,” Surface Science, vol. 525, no. 1–3, pp. L103–L108, 2003. [14] P. M. Ajayan, O. Stephan, C. Colliex, and D. Trauth, “Aligned carbon nanotube arrays formed by cutting a polymer resinnanotube composite,” Science, vol. 265, no. 5176, pp. 1212– 1214, 1994. [15] M. S. P. Shaﬀer and A. H. Windle, “Fabrication and characterization of carbon nanotube/poly(vinyl alcohol) composites,” Advanced Materials, vol. 11, no. 11, pp. 937–941, 1999. [16] X. Gong, J. Liu, S. Baskaran, R. D. Voise, and J. S. Young, “Surfactant-assisted processing of carbon nanotube/polymer composites,” Chemistry of Materials, vol. 12, no. 4, pp. 1049– 1052, 2000. [17] S. Kumar, H. Doshi, M. Srinivasarao, J. O. Park, and D. A. Schiraldi, “Fibers from polypropylene/nano carbon fiber composites,” Polymer, vol. 43, no. 5, pp. 1701–1703, 2002. [18] X. Tong, X.-J. He, and H.-M. Cheng, “Eﬀect of carbon nanotubes on mechanical properties and crystallization process of high density polyethylene,” New Carbon Materials, vol. 19, no. 4, pp. 261–267, 2004. [19] D. Qian, E. C. Dickey, R. Andrews, and T. Rantell, “Load transfer and deformation mechanisms in carbon nanotubepolystyrene composites,” Applied Physics Letters, vol. 76, no. 20, pp. 2868–2870, 2000. [20] C. Bower, R. Rosen, L. Jin, J. Han, and O. Zhou, “Deformation of carbon nanotubes in nanotube-polymer composites,” Applied Physics Letters, vol. 74, no. 22, pp. 3317–3319, 1999. [21] P. M. Ajayan, L. S. Schadler, C. Giannaris, and A. Rubio, “Single-walled carbon nanotube-polymer composites: strength and weakness,” Advanced Materials, vol. 12, no. 10, pp. 750–753, 2000. [22] B. Ni and S. B. Sinnott, “Tribological properties of carbon nanotube bundles predicted from atomistic simulations,” Surface Science, vol. 487, no. 1–3, pp. 87–96, 2001. [23] Y. Hu, I. Jang, and S. B. Sinnott, “Modification of carbon nanotube-polystyrene matrix composites through polyatomic-ion beam deposition: predictions from molecular dynamics simulations,” Composites Science and Technology, vol. 63, no. 11, pp. 1663–1669, 2003. [24] Y. L. Chen, B. Liu, X. Q. He, Y. Huang, and K. C. Hwang, “Failure analysis and the optimal toughness design of carbon nanotube-reinforced composites,” Composites Science and Technology, vol. 70, no. 9, pp. 1360–1367, 2010. Journal of Nanomaterials [25] R. Z. Ma, J. Wu, B. Q. Wei, J. Liang, and D. H. Wu, “Processing and properties of carbon nanotubes-nano-SiC ceramic,” Journal of Materials Science, vol. 33, no. 21, pp. 5243– 5246, 1998. [26] E. Flahaut, A. Peigney, CH. Laurent, CH. Marlière, F. Chastel, and A. Rousset, “Carbon nanotube-metal-oxide nanocomposites: microstructure, electrical conductivity and mechanical properties,” Acta Materialia, vol. 48, no. 14, pp. 3803–3812, 2000. [27] A. Peigney, C. Laurent, O. Dumortier, and A. Rousset, “Carbon nanotubes-Fe-alumina nanocomposites. Part I: influence of the Fe content on the synthesis of powders,” Journal of the European Ceramic Society, vol. 18, no. 14, pp. 1995–1104, 1998. [28] C. Laurent, A. Peigney, O. Dumortier, and A. Rousset, “Carbon nanotubes-Fe-Alumina nanocomposites. Part II: microstructure and mechanical properties of the hot-Pressed composites,” Journal of the European Ceramic Society, vol. 18, no. 14, pp. 2005–2013, 1998. [29] A. Peigney, CH. Laurent, and A. Rousset, “Synthesis and characterization of alumina matrix nanocomposites containing carbon nanotubes,” Key Engineering Materials, no. 136, pp. 743–746, 1997. [30] X. Chen, J. Xia, J. Peng, W. Li, and S. Xie, “Carbon-nanotube metal-matrix composites prepared by electroless plating,” Composites Science and Technology, vol. 60, no. 2, pp. 301–306, 2000. [31] C. L. Xu, B. Q. Wei, R. Z. Ma, J. Liang, X. K. Ma, and D. H. Wu, “Fabrication of aluminum-carbon nanotube composites and their electrical properties,” Carbon, vol. 37, no. 5, pp. 855– 858, 1999. [32] H. L. Cox, “The elasticity and strength of paper and other fibrous materials,” British Journal of Applied Physics, vol. 3, no. 1, pp. 72–79, 1952. [33] C. T. Chon and C. T. Sun, “Stress distributions along a short fibre in fibre reinforced plastics,” Journal of Materials Science, vol. 15, no. 4, pp. 931–938, 1980. [34] P. Lawrence, “Some theoretical considerations of fibre pull-out from an elastic matrix,” Journal of Materials Science, vol. 7, no. 1, pp. 1–6, 1972. [35] D. B. Marshall, B. N. Cox, and A. G. Evans, “The mechanics of matrix cracking in brittle-matrix fiber composites,” Acta Metallurgica, vol. 33, no. 11, pp. 2013–2021, 1985. [36] J. W. Hutchinson and H. M. Jensen, “Models of fiber debonding and pullout in brittle composites with friction,” Mechanics of Materials, vol. 9, no. 2, pp. 139–163, 1990. [37] B. Budiansky, A. G. Evans, and J. W. Hutchinson, “Fibermatrix debonding eﬀects oncracking in aligned fiber ceramic composites,” International Journal of Solids and Structures, vol. 32, no. 3-4, pp. 315–328, 1995. [38] T. L. Anderson, Fracture Mechanics: Fundamentals and Applications, CRC Press LLC, Boca Raton, Fla, USA, 1995. [39] H. Tada, P. C. Paris, and G R. Irwin, The Stress Analysis of Cracks Handbook, ASME Press, New York, NY, USA, 3rd edition, 2000. [40] Z. Xia, L. Riester, W. A. Curtin et al., “Direct observation of toughening mechanisms in carbon nanotube ceramic matrix composites,” Acta Materialia, vol. 52, no. 4, pp. 931–944, 2004. [41] Z. Xia and W. A. Curtin, “Tough-to-brittle transitions in ceramic-matrix composites with increasing interfacial shear stress,” Acta Materialia, vol. 48, no. 20, pp. 4879–4892, 2000. [42] W. Zhou, Y. Huang, B. Liu et al., “Self-folding of single- and multiwall carbon nanotubes,” Applied Physics Letters, vol. 90, no. 7, Article ID 73107, 2007. 9